Bioimaging Tools Based on Polyelectrolyte Microcapsules Encoded with Fluorescent Semiconductor Nanoparticles: Design and Characterization of the Fluorescent Properties
- 422 Downloads
Fluorescent imaging is a widely used technique for detecting and monitoring the distribution, interaction, and transformation processes at molecular, cellular, and tissue level in modern diagnostic and other biomedical applications. Unique photophysical properties of fluorescent semiconductor nanocrystals “quantum dots” (QDs) make them advanced fluorophores for fluorescent labeling of biomolecules or optical encoding of microparticles to be used as bioimaging and theranostic agents in targeted delivery, visualization, diagnostics, and imaging. This paper reports on the results of development of an improved approach to the optical encoding of polyelectrolyte microcapsules with stable, covered with the multifunctional polyethyleneglycol derivatives water-soluble QDs, as well as characterization of the optical properties, morphological and structural properties of the encoded microcapsules. The embedding of QDs into the polymer microcapsule membrane through layer-by-layer deposition on a preliminarily formed polymeric polyelectrolyte shell makes it possible to obtain bright fluorescent particles with an adapted charge and size distribution that are distinctly discernible by flow cytometry as individual homogeneous populations. The fluorescent microcapsules developed can be used in further designing bioimaging and theranostic agents sensitive to various external stimuli along with photoexcitation.
KeywordsPolymer microcapsules Polyelectrolytes Quantum dots Bioimaging
Bovine serum albumin
Polycation poly(allylamine hydrochloride)
Polyanion poly(sodium 4-styrenesulfonate)
Development of fluorescent polymer micro- and nanoparticles to be used as carriers for targeted delivery of drugs, protein, and nucleic acid molecules is of special interest in the field of bioimaging and theranostic agents design [1, 2, 3]. Quantum dots (QDs) are 2- to 10-nm semiconductor colloidal crystals with the fluorescence peak wavelength depending on their physical size. A wide absorption spectrum and a narrow, symmetrical fluorescence spectrum with its position depending on nanoparticle size allow a single radiation source to be used for exciting fluorescence in a set of QDs with different fluorescence bands, which can be used for multiplexed detection. Therefore, QDs are very attractive and promising advanced fluorophores for diagnostics and imaging .
The use of polyelectrolyte microcapsules as carriers of various functional components makes it possible to develop a system responding to various physical (ultrasound, magnetic field, laser, or optical radiation) or chemical (pH, ionic strength of the microenvironment, and polarity of solvents) stimuli [5, 6]. The polyelectrolyte microcapsules are obtained using layer-by-layer deposition of oppositely charged polymeric polyelectrolytes onto a spherical matrix. The subsequent dissolution of the matrix yields a hollow structure whose stable polymer membrane consists of an interpolymer complex of polyelectrolytes [7, 8, 9]. The technique of layer-by-layer adsorption of polyelectrolytes allows various functional components, including magnetic, metal (gold or silver), or fluorescent (e.g., QDs) nanoparticles to be incorporated into the polymer membrane and the thickness of the membrane to be controlled as it is formed [10, 11].
Fluorescently labeled microcapsules are promising bioimaging agents that can be used to monitor their in vitro and in vivo transport and delivery [12, 13]. In the available methods of fluorescent labeling (optical encoding) of microcapsules, polymers are conjugated or physically mixed with fluorescent labels [14, 15]. The fluorescent components determining the optical properties of the microcapsules can also be incorporated inside them via co-precipitation of polymers labeled with fluorescent dyes during preparation of the matrix microparticles, e.g., calcium carbonate microspherolites . They can also be encapsulated after the matrix is removed; for this purpose, diffusion of low and high molecular weight compounds through the polymer membrane is ensured by increasing the ionic strength or pH of the microenvironment. However, optical encoding of polyelectrolyte microcapsules with fluorescent nanocrystals is more promising due to their unique optical properties and effectiveness in bioimaging .
The known methods of encoding by incorporating QDs into the polymer membrane of polyelectrolyte microcapsules employ QDs water-solubilized with a low molecular weight ligand, e.g., thioglycolic acid or cysteine [18, 19]. The goal of this study was to develop highly stable fluorescent polyelectrolyte microcapsules optically encoded with water-soluble CdSe/ZnS (core/shell) QDs whose surface was additionally modified with a thiol derivative of polyethylene glycol (PEG) containing a carboxyl terminal group and to estimate the fluorescence and structure characteristics of the resultant fluorescent microcapsules.
The Aim, Design, and Setting of the Study
Fabrication of QD-Encoded Polyelectrolyte Microcapsules
CdSe/ZnS (core/shell) QDs with a fluorescence maximum at 590 nm coated with trioctylphosphine oxide (TOPO) were synthesized by Dr. P. Samokhvalov in the Laboratory of Nano-Bioengineering of NRNU MEPhI (Moscow, Russia). The QD purification and solubilization were carried as described earlier [20, 21]. TOPO was removed from the QD surface by dissolving the QDs in chloroform and subsequently precipitating them with methanol; the procedure was repeated three times. After that, the QDs were dissolved in chloroform again and precipitated with a cysteine solution in methanol at a QD-to-cysteine mass ratio of 1:0.13. The QD precipitate was washed of excess cysteine with methanol and dried in a vacuum concentrator. The dried QDs were resuspended in water with addition of 0.1 M sodium hydroxide. Afterwards, the dispersion was sonicated using ultrasound bath and filtered (pore size, 0.22 μm). To the resultant dispersion, a thiol derivative of PEG containing a terminal carboxyl group was added at a mass ratio of 1:4.6. The mixture was incubated overnight at 4 °C and PEGylated QDs were purified using gel filtration chromatography. The QD content of the samples obtained was determined spectrophotometrically at the wavelength of the first exciton. Solubilized QDs were characterized by hydrodynamic diameter and ζ-potential using dynamic light scattering and laser Doppler micro-electrophoresis by means of Zetasizer Nano ZS (Malvern, UK).
The QD encoding was performed using a modified technique of layer-by-layer deposition of oppositely charged polycation and polyanion polymers, as well as water-soluble QDs functionalized with carboxylated thiol derivatives of PEG, onto the surface of calcium carbonate microparticles obtained as described earlier . The polymeric polyelectrolyte layers were formed out of the polycation poly(allylamine hydrochloride) (PAH) and the polyanion poly(sodium 4-styrenesulfonate) (PSS) or polyacrylic acid (PAA); the fluorophores were water-soluble PEGylated CdSe/ZnS QDs with a fluorescence peak at a wavelength of 590 nm, a ζ-potential of -26.7 ± 0.8 mV, and a hydrodynamic diameter from 18.7 to 23.3 nm. During the QD-encoded microcapsule, manufacturing process after each layer deposition the microparticle surface charge (ζ-potential) was controlled using laser Doppler micro-electrophoresis.
The calcium carbonate microparticles were resuspended in ultrapure water, and 0.5 mL of a 2 mg/mL PAH solution in 0.5 M NaCl was added. The suspension was sonicated in an ultrasound bath and incubated for 20 min while stirring at room temperature. After that, the excess polymer was washed off by centrifugation followed by resuspension in MilliQ water. For applying the next layer, consisting of the polymeric polyanion, the microbeads were resuspended in 0.5 mL of ultrapure water, and the suspension was mixed with 0.5 mL of a 2 mg/mL PSS solution in 0.5 M NaCl, sonicated in an ultrasound bath for 60 s, incubated for 20 min while stirring at room temperature, and washed of the excess polymer as described above. The washing of the microparticles after each stage of polyelectrolyte application was repeated three times. Before the encoding, five polyelectrolyte layers were applied onto the calcium carbonate microparticles, the fifth layer consisting of the polycation. After that, solubilized QDs were added, and the mixture was incubated while permanently stirring for 80 min. Then, six successive layers of oppositely charged polymers were applied, the sixth one consisting of polyanion PSS or PAA. Hollow polyelectrolyte microcapsules encoded with QDs were obtained by dissolving the calcium carbonate cores of the resultant shelled microbeads by washing them with 0.2 M disodium ethylenediaminetetraacetate (EDTA) (pH 6.5). After that, the microcapsule surface was additionally modified with bovine serum albumin (BSA) (Sigma-Aldrich, USA) by dispersing the microparticles in a 50 mM phosphate buffer solution (pH 7.4) containing 1% of BSA and subsequently incubating at 4 °C for 12 h in the dark. Shortly before use, the suspension of hollow microcapsules was washed of excess BSA five times with a 50 mM phosphate buffer solution (pH 7.4). The obtained polyelectrolyte microcapsules were stored at 4 °C in the dark.
Optical and Fluorescence Microscopies of the QD-Encoded Polyelectrolyte Microcapsules
The morphology and size distribution of the microparticles were analyzed using optical and fluorescence microscopies. In order to estimate the size distribution of the microparticles, we fixed 5 μL of the microparticle suspension in 10 μL of 50% glycerol on a slide. The samples were examined by means of an Axio Observer 3 microscope (Carl Zeiss, Germany) with an LD A-Plan 40x/0.55 M27 lens in a light field. Fluorescent images were obtained using an HBO 100 mercury illuminator (Burner Mercury) with an XF115-2 FITC longpass filter set, including a 505DRLP dichroic filter, a 475AF40 excitation filter, and a 510ALP emission filter (Omega Optical, USA), an EC Plan-Neofluar 100x/1.30 Oil Iris M27 lens (WD = 0.20 mm), a numerical aperture adjustable from 0.7 to 1.3, and Immersol 518F immersion oil (Carl Zeiss, Germany).
The morphological characteristics of the obtained microcapsules were studied in sections of the optically encoded polyelectrolyte microcapsules with a BSA-free surface fixed in epoxy embedding medium. For this purpose, the microcapsule suspension was sequentially dehydrated with 30, 50, 70, and 95% aqueous ethanol solutions and then treated with absolute ethanol (Acros Organics, USA) three times to ensure complete dehydration. Each stage of dehydration lasted for 15 min. Dehydrated samples of microcapsules were transferred to a 1:1 epoxy–ethanol mixture for 12 h and then to a 3:1 epoxy–ethanol mixture for 3 h. Then, the samples were transferred to a clean embedding epoxy media, and epoxy blocks were polymerized at 45 °C for 12 h and at 60 °C for 72 h. Then, 150-nm sections were cut from these blocks containing fluorescent QD-encoded polyelectrolyte microcapsules by means of a Leica EM UC6 ultramicrotome (Leica Microsystems, Austria) equipped with an Ultra AFM 35 diamond knife (Diatome, Switzerland) 2.0 mm in width. The sections were transferred onto a slide and examined under an Axio Vert.A1 fluorescent microscope (Carl Zeiss, Germany) using an HBO 100 mercury illuminator (Burner Mercury) for excitation and a 45 HQ TexasRed fluorescent filter set (d = 25 shift free (E), a 560/40 excitation BP, a FT 585 beam splitter, and a 630/75 emission BP) (Carl Zeiss, Germany) for recording fluorescence. Fluorescent images were obtained using a Carl Zeiss EC Plan-Neofluar100x/1.30 Oil Ph3 lens and Immersol 518F immersion oil (Carl Zeiss, Germany). The images were analyzed and processed using the Zen (Carl Zeiss, Germany) and Image J 1.48 v (USA) software.
Fluorescence Characteristics of the QD-Encoded Microcapsules
The fluorescence characteristics of the original QDs used for encoding and the QD-encoded microcapsules were analyzed using an Infinite 200 PRO multimodal plate reader (TECAN, Switzerland). Before the measurements, the plate with wells containing suspensions of QD-encoded microcapsules and microspheres was centrifuged using a 5810 R centrifuge (Eppendorf, USA) with an А-2-DWP rotor at 2630×g for 20 min. The fluorescence maxima of free QDs and QDs embedded in the polymer shell of the polyelectrolyte microcapsules were determined at an excitation wavelength of 480 nm; bottom-scanning mode was used for analysis of the samples.
An FACSCanto II flow cytometer (Becton Dickinson, USA) equipped with a blue (488 nm) argon laser as an excitation source was used to analyze the samples of the original calcium carbonate microparticles, the microparticles with the QD-containing polyelectrolyte shell, and the QD-encoded hollow microcapsules. We analyzed 0.5-mL aliquots of a suspension containing 106 microbeads/microcapsules; the number of collected events was 2500. The fluorescence intensity was recorded in the standard forward-scattered light (FSC), side-scattered light (SSC), and phycoerythrin (PE, 585/42 nm) channels. The data were processed using the FACSDiva software (Becton Dickinson, USA).
We used carboxylated thiol derivatives of PEG containing a 12-monomer PEG spacer (Thermo Fisher Scientific, USA), poly(allylamine hydrochloride) (PAH) with Mw ≈ 15,000 Da (Sigma-Aldrich, Japan), poly(sodium 4-styrenesulfonate) (PSS) with Mw ≈ 70,000 Da (Sigma-Aldrich, USA), and polyacrylic acid (PAA) with Mw ≈ 15,000 Da (Sigma-Aldrich, USA). Sodium carbonate, calcium chloride, ethylenediaminetetraacetic acid disodium salt dehydrate, bovine serum albumin (BSA), epoxy embedding medium, and other reagents were from Sigma-Aldrich (USA). All working solutions were prepared using MilliQ water (18.2 mΩ cm) obtained by means of a Direct-Q water purification system (Millipore, France) and filtered through filters with a pore size of 0.22 μm.
The MS Office Excel 2007 and Origin Pro 2015 software packages were used for statistical analysis of the data. The results are presented as the means and standard deviations for three independent experiments.
Results and Discussion
Development of QD-Encoded Polyelectrolyte Microcapsules
Hollow microcapsules containing immobilized QDs in their polymer membrane are obtained by dissolving the calcium carbonate microparticles with 0.2 M EDTA (pH 6.5) and formation of the water-soluble complex of calcium salt of ethylenediaminetetraacetic acid, whose diffusion through the polymer membrane results in formation of cavities inside the microcapsules. For obtaining QD-encoded polyelectrolyte microcapsules with a BSA-modified surface, the PAA polyanion is layered onto the 11th layer of the PAH polycation. PAA is used because of its value of the dissociation constant upon interaction with the microcapsule surface. pKa value of PAA (pKa ≈ 4.7) is lower and, hence, more acidic compared to PSS (pKa ≈ 7.5) [25, 26], which results in a higher ζ-potential of the microcapsule surface. The charge of the PAA-modified surface facilitates BSA passive adsorption due to electrostatic interaction between BSA and PAA. However, assembly between PAA and BSA results in microcapsule negative surface charge decrease (Fig. 1b). After BSA deposition onto the microcapsule surface, the shielding of negatively charged PAA layer by electrostatically positive amino groups of BSA occurs, hence, the ζ-potential of the BSA-coated QD-encoded microcapsules is likely primary determined by electrostatic behavior of BSA as an outer microcapsule coating .
The water-soluble PEGylated QDs are characterized by a narrow size distribution, the absence of aggregations in the dispersion, and a high colloidal stability. This is likely to ensure homogeneous adsorption of QDs on the microbead surface and facilitate effective encoding and, hence, obtaining bright fluorescent microcapsules (Fig. 1c).
The use of proteins, such as BSA, for surface modification makes the polymer microcapsules more biocompatible and more resistant to adhesion with one another. This also ensures temporary passivation of the microcapsule surface, which is important for the subsequent study of the microcapsules formed by PAH–PSS or PAH–PAA interpolymer complexes in terms of in vitro interaction with cells and in vivo behavior [27, 28, 29].
The Fluorescence and Structure Characteristics of the QD-Encoded Polyelectrolyte Microcapsules
Developed technique for obtaining QD-encoded polyelectrolyte microcapsules ensures effective optical encoding. The fabricated polymer microcapsules are characterized by an optimal size distribution and high fluorescence intensity to be used for their efficient detection by commercial flow cytometers and confocal microscopes. Therefore, the designed microcapsules are potential fluorescent agents for in vitro and in vivo bioimaging. Further development of the versatile microcapsule-based platform would be aimed to proposition of novel bioimaging and theranostic tools based on fluorescent QD-encoded microparticles which are responsive to different external physical or chemical stimuli along with photoexcitation.
We thank Dr. Pavel Samokhvalov for providing of as-synthetized QDs and Vladimir Ushakov for the help in technical preparation of the manuscript.
This study was supported by the Ministry of Education and Science of the Russian Federation, State Contract no. 16.1034.2017/ПЧ.
Availability of Data and Materials
The datasets generated during and/or analyzed during the current study are available from the corresponding authors on reasonable request.
GN, IN, and AS designed the study and all experiments. GN developed procedures and synthesized polyelectrolyte microcapsules encoded with QDs. AE, OA, and IA performed optical and structural characterization of QDs and fluorescent microcapsules. GN, IN, and AS wrote the manuscript. All authors discussed the results and commented on the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
- 9.Tacheva B, Parvanova B, Sandev N, Zarkov I, Karabaliev M, Bäumler H, Georgieva R (2015) Polyelectrolyte microcapsules with potential for cellular delivery of drugs. Sci Technol 5:411–416Google Scholar
- 18.Sukhanova A, Venteo L, Devy J et al (2002) Highly stable fluorescent nanocrystals as a novel class of labels for immunohistochemical analysis of paraffin-embedded tissue sections. Lab Investig 82:1259–1262. https://doi.org/10.1097/01.LAB.0000027837.13582.E8 CrossRefGoogle Scholar
- 20.Brazhnik K, Sokolova Z, Baryshnikova M, Bilan R, Efimov A, Nabiev I, Sukhanova A (2015) Quantum dot-based lab-on-a-bead system for multiplexed detection of free and total prostate-specific antigens in clinical human serum samples. Nanomedicine: NBM 11:1065–1075. https://doi.org/10.1016/j.nano.2015.03.003 CrossRefGoogle Scholar
- 22.Nifontova G, Zvaigzne M, Baryshnikova M et al (2018) Next-generation theranostic agents based on polyelectrolyte microcapsules encoded with semiconductor nanocrystals: development and functional characterization. Nanoscale Res Lett 13(30):1–12. https://doi.org/10.1186/s11671-018-2447-z CrossRefGoogle Scholar
- 33.Mcdonald DM, Baluk P (2002) Significance of blood vessel leakiness in cancer. Cancer Res 62:5381–5385Google Scholar
- 39.Gaigalas AK, Wang L (2008) Measurement of the fluorescence quantum yield using a spectrometer with an integrating sphere detector. J Res Natl Inst Stand Technol 113(1):17–28. https://www.ncbi.nlm.nih.gov/pmc/articles/PMC4654612/
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.